#------------------------------------------------------------------------------
#$Date: 2016-03-23 16:25:09 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179376 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/73/4327302.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4327302
loop_
_publ_author_name
'Anne Dolbecq'
'Laurent Lisnard'
'Pierre Mialane'
'Jérôme Marrot'
'Marc Bénard'
'Marie-Madeleine Rohmer'
'Francis Sécheresse'
_publ_section_title
;
 Synthesis and Characterization of Octa- and Hexanuclear Polyoxomolybdate
 Wheels: Role of the Inorganic Template and of the Counterion
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5898
_journal_page_last               5910
_journal_paper_doi               10.1021/ic060410+
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'C6 H82 Li14 Mo8 O86 P12'
_chemical_formula_weight         2767.04
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                101.2000(10)
_cell_angle_beta                 107.4770(10)
_cell_angle_gamma                108.0670(10)
_cell_formula_units_Z            1
_cell_length_a                   11.85910(10)
_cell_length_b                   11.98120(10)
_cell_length_c                   16.0452(2)
_cell_measurement_temperature    293(2)
_cell_volume                     1960.79(4)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.867
_diffrn_measured_fraction_theta_max 0.867
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0244
_diffrn_reflns_av_sigmaI/netI    0.0425
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            13706
_diffrn_reflns_theta_full        29.67
_diffrn_reflns_theta_max         29.67
_diffrn_reflns_theta_min         1.40
_exptl_absorpt_coefficient_mu    1.602
_exptl_absorpt_correction_T_max  0.7400
_exptl_absorpt_correction_T_min  0.4466
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.310
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             1364
_exptl_crystal_size_max          0.60
_exptl_crystal_size_mid          0.40
_exptl_crystal_size_min          0.20
_refine_diff_density_max         2.581
_refine_diff_density_min         -1.313
_refine_diff_density_rms         0.179
_refine_ls_extinction_coef       0.0015(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.103
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     553
_refine_ls_number_reflns         9767
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.103
_refine_ls_R_factor_all          0.0629
_refine_ls_R_factor_gt           0.0528
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0602P)²+13.0206P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1359
_refine_ls_wR_factor_ref         0.1440
_reflns_number_gt                8310
_reflns_number_total             9767
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0604102Bsi20060310_054443_6.cif
_cod_data_source_block           4c
_cod_original_cell_volume        1960.72(3)
_cod_database_code               4327302
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.34290(4) 0.80656(4) 0.18743(3) 0.02139(11) Uani 1 1 d .
Mo2 Mo -0.13674(4) 0.35919(4) 0.18693(3) 0.02119(11) Uani 1 1 d .
Mo3 Mo 0.34602(4) 0.81471(4) 0.34898(3) 0.02365(12) Uani 1 1 d .
Mo4 Mo 0.01798(4) 0.50817(4) 0.34802(3) 0.02364(12) Uani 1 1 d .
P1 P 0.12797(12) 0.54078(12) 0.17520(9) 0.0195(2) Uani 1 1 d .
P2 P 0.24773(13) 0.88401(12) -0.00155(9) 0.0216(3) Uani 1 1 d .
P3 P 0.39997(13) 0.72507(12) 0.00035(9) 0.0212(3) Uani 1 1 d .
P4 P 0.17256(15) 0.31041(14) 0.09334(11) 0.0281(3) Uani 1 1 d .
P5 P 0.16880(14) 0.80750(13) 0.47814(10) 0.0262(3) Uani 1 1 d .
P6 P 0.32463(15) 0.65498(14) 0.49794(10) 0.0280(3) Uani 1 1 d .
O1 O 0.2181(4) 0.8278(4) 0.0718(3) 0.0256(8) Uani 1 1 d .
O2 O -0.1151(4) 0.5243(3) 0.2503(3) 0.0241(7) Uani 1 1 d .
O3 O 0.0865(4) 0.3151(4) 0.0030(3) 0.0343(9) Uani 1 1 d .
O4 O 0.4664(4) 0.9432(4) 0.2147(3) 0.0319(9) Uani 1 1 d .
O5 O 0.0512(4) 0.6870(4) 0.4175(3) 0.0289(8) Uani 1 1 d .
O6 O 0.2410(4) 0.8549(4) 0.2505(3) 0.0250(8) Uani 1 1 d .
O7 O 0.2715(4) 0.6267(3) -0.0734(3) 0.0251(8) Uani 1 1 d .
O8 O 0.4086(4) 0.7241(4) 0.2709(3) 0.0245(7) Uani 1 1 d .
O9 O 0.0239(4) 0.3655(3) 0.2697(3) 0.0241(7) Uani 1 1 d .
O10 O 0.1405(4) 0.7983(3) -0.0960(3) 0.0254(8) Uani 1 1 d .
O11 O -0.0132(3) 0.4525(3) 0.1202(2) 0.0212(7) Uani 1 1 d .
O12 O 0.4074(4) 0.7156(3) 0.0963(3) 0.0246(8) Uani 1 1 d .
O13 O 0.2590(4) 1.0147(4) 0.0149(3) 0.0342(9) Uani 1 1 d .
O14 O 0.2016(4) 0.5413(4) 0.4348(3) 0.0299(8) Uani 1 1 d .
O15 O 0.2350(4) 0.8582(4) 0.4165(3) 0.0285(8) Uani 1 1 d .
O16 O 0.5145(4) 0.7168(4) -0.0180(3) 0.0317(9) Uani 1 1 d .
O17 O 0.2896(4) 0.2883(4) 0.0905(3) 0.0369(10) Uani 1 1 d .
O18 O 0.4762(4) 0.9460(4) 0.4074(3) 0.0349(9) Uani 1 1 d .
O19 O 0.0941(5) 0.2025(4) 0.1230(4) 0.0409(11) Uani 1 1 d .
O20 O 0.1504(4) 0.6147(3) 0.2729(2) 0.0228(7) Uani 1 1 d .
O21 O 0.3902(4) 0.7168(4) 0.4394(3) 0.0293(8) Uani 1 1 d .
O22 O -0.2490(4) 0.2675(4) 0.2161(3) 0.0317(9) Uani 1 1 d .
O23 O 0.1694(4) 0.6273(3) 0.1214(2) 0.0228(7) Uani 1 1 d .
O24 O -0.0233(4) 0.7581(4) 0.2239(3) 0.0378(10) Uani 1 1 d .
O25 O 0.2916(5) 0.4018(4) -0.0689(4) 0.0410(11) Uani 1 1 d .
O26 O -0.0633(5) 0.4413(4) 0.4062(3) 0.0379(10) Uani 1 1 d .
O27 O 0.1307(5) 0.8997(4) 0.5271(3) 0.0381(10) Uani 1 1 d .
O28 O 0.5175(5) 0.5541(5) 0.1388(4) 0.0486(12) Uani 1 1 d .
O29 O 0.4124(5) 0.6170(5) 0.5648(3) 0.0438(11) Uani 1 1 d .
C1 C 0.2249(5) 0.4507(5) 0.1855(4) 0.0268(11) Uani 1 1 d .
H1A H 0.3101 0.5032 0.1933 0.032 Uiso 1 1 calc R
H1B H 0.2323 0.4295 0.2413 0.032 Uiso 1 1 calc R
C2 C 0.3948(5) 0.8726(5) -0.0025(4) 0.0236(10) Uani 1 1 d .
H2A H 0.4658 0.9367 0.0501 0.028 Uiso 1 1 calc R
H2B H 0.4057 0.8871 -0.0572 0.028 Uiso 1 1 calc R
C3 C 0.2808(6) 0.7670(6) 0.5573(4) 0.0319(12) Uani 1 1 d .
H3A H 0.3570 0.8405 0.5953 0.038 Uiso 1 1 calc R
H3B H 0.2425 0.7339 0.5971 0.038 Uiso 1 1 calc R
OW1 O -0.0279(7) 0.9390(7) 0.3674(5) 0.075(2) Uani 1 1 d .
OW2 O 0.1317(9) 1.0889(6) -0.1229(5) 0.080(2) Uani 1 1 d .
OW3 O 0.4838(7) 1.1972(8) 0.2038(6) 0.086(2) Uani 1 1 d .
OW4 O -0.3522(7) 0.4730(8) 0.2733(5) 0.075(2) Uani 1 1 d .
OW5 O 0.3153(7) 1.1184(6) 0.4426(5) 0.075(2) Uani 1 1 d .
OW6 O 0.0741(9) 0.1942(9) 0.3484(7) 0.107(3) Uani 1 1 d .
OW7 O -0.1681(8) 0.6674(9) 0.4631(7) 0.108(3) Uani 1 1 d .
OW8 O 0.7689(11) 1.0179(11) 0.2517(6) 0.120(4) Uani 1 1 d .
OW9 O 0.1317(12) 0.2557(12) -0.0996(8) 0.059(3) Uani 0.50 1 d P
OW10 O 0.5294(10) 0.5876(10) 0.3853(9) 0.123(4) Uani 1 1 d .
OW11 O 0.1522(15) 1.0312(14) 0.2099(10) 0.073(4) Uiso 0.50 1 d P
OW12 O 0.6900(10) 0.8110(11) 0.3460(10) 0.062(3) Uani 0.50 1 d P
OW13 O 0.6687(12) 0.6506(11) 0.6092(11) 0.067(4) Uani 0.50 1 d P
OW14 O 0.646(2) 0.709(2) 0.6831(18) 0.141(8) Uiso 0.50 1 d P
OW15 O 0.2438(18) 1.0902(17) 0.2367(12) 0.089(5) Uiso 0.50 1 d P
Li1 Li 0.0678(11) 0.6539(10) 0.0121(7) 0.032(2) Uani 1 1 d .
Li2 Li 0.3762(11) 0.1819(10) 0.0765(9) 0.041(3) Uani 1 1 d .
Li3 Li 0.5957(12) 0.6105(12) -0.0468(9) 0.044(3) Uani 1 1 d .
Li4 Li -0.3457(19) 0.5257(19) 0.3981(15) 0.078(5) Uani 1 1 d .
Li5 Li 0.228(2) 1.170(2) 0.342(2) 0.103(8) Uani 1 1 d .
Li6 Li 0.180(2) 1.026(2) 0.6349(15) 0.034(4) Uiso 0.50 1 d P
Li7 Li 0.090(5) 0.938(5) 0.641(4) 0.105(14) Uiso 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Mo1 O8 105.35(19) . .
O4 Mo1 O6 102.07(19) . .
O8 Mo1 O6 95.74(16) . .
O4 Mo1 O12 91.56(18) . .
O8 Mo1 O12 86.51(15) . .
O6 Mo1 O12 165.00(16) . .
O4 Mo1 O1 95.63(18) . .
O8 Mo1 O1 158.31(16) . .
O6 Mo1 O1 85.02(15) . .
O12 Mo1 O1 87.47(15) . .
O4 Mo1 O23 168.11(17) . .
O8 Mo1 O23 84.53(15) . .
O6 Mo1 O23 83.14(15) . .
O12 Mo1 O23 82.31(14) . .
O1 Mo1 O23 74.02(14) . .
O4 Mo1 Mo3 99.14(14) . .
O8 Mo1 Mo3 49.08(11) . .
O6 Mo1 Mo3 48.73(11) . .
O12 Mo1 Mo3 135.59(10) . .
O1 Mo1 Mo3 133.39(11) . .
O23 Mo1 Mo3 92.33(9) . .
O4 Mo1 Li1 133.3(2) . .
O8 Mo1 Li1 120.0(2) . .
O6 Mo1 Li1 84.7(2) . .
O12 Mo1 Li1 81.3(2) . .
O1 Mo1 Li1 38.4(2) . .
O23 Mo1 Li1 35.8(2) . .
Mo3 Mo1 Li1 118.01(18) . .
O22 Mo2 O2 102.83(18) . .
O22 Mo2 O9 103.68(19) . .
O2 Mo2 O9 96.02(15) . .
O22 Mo2 O7 94.73(19) . 2_565
O2 Mo2 O7 85.31(15) . 2_565
O9 Mo2 O7 160.70(16) . 2_565
O22 Mo2 O10 90.95(18) . 2_565
O2 Mo2 O10 165.23(16) . 2_565
O9 Mo2 O10 85.69(15) . 2_565
O7 Mo2 O10 88.30(15) 2_565 2_565
O22 Mo2 O11 168.42(17) . .
O2 Mo2 O11 85.45(15) . .
O9 Mo2 O11 83.20(15) . .
O7 Mo2 O11 77.70(14) 2_565 .
O10 Mo2 O11 80.18(14) 2_565 .
O22 Mo2 Mo4 98.85(14) . .
O2 Mo2 Mo4 49.08(11) . .
O9 Mo2 Mo4 48.89(11) . .
O7 Mo2 Mo4 134.21(10) 2_565 .
O10 Mo2 Mo4 134.59(10) 2_565 .
O11 Mo2 Mo4 92.70(9) . .
O18 Mo3 O6 104.2(2) . .
O18 Mo3 O8 101.05(19) . .
O6 Mo3 O8 94.98(15) . .
O18 Mo3 O15 96.05(19) . .
O6 Mo3 O15 84.02(16) . .
O8 Mo3 O15 162.57(17) . .
O18 Mo3 O21 96.9(2) . .
O6 Mo3 O21 157.90(16) . .
O8 Mo3 O21 87.41(16) . .
O15 Mo3 O21 87.20(16) . .
O18 Mo3 Mo1 97.48(15) . .
O6 Mo3 Mo1 48.56(11) . .
O8 Mo3 Mo1 48.46(11) . .
O15 Mo3 Mo1 132.54(11) . .
O21 Mo3 Mo1 135.45(12) . .
O26 Mo4 O9 101.2(2) . .
O26 Mo4 O2 102.8(2) . .
O9 Mo4 O2 95.21(15) . .
O26 Mo4 O5 95.3(2) . .
O9 Mo4 O5 163.11(17) . .
O2 Mo4 O5 84.42(15) . .
O26 Mo4 O14 98.6(2) . .
O9 Mo4 O14 86.87(16) . .
O2 Mo4 O14 157.61(17) . .
O5 Mo4 O14 87.22(16) . .
O26 Mo4 O20 175.95(18) . .
O9 Mo4 O20 80.72(14) . .
O2 Mo4 O20 80.48(14) . .
O5 Mo4 O20 82.57(15) . .
O14 Mo4 O20 77.87(15) . .
O26 Mo4 Mo2 96.93(15) . .
O9 Mo4 Mo2 48.61(11) . .
O2 Mo4 Mo2 48.52(11) . .
O5 Mo4 Mo2 132.91(11) . .
O14 Mo4 Mo2 134.95(12) . .
O20 Mo4 Mo2 87.01(9) . .
O23 P1 O11 108.8(2) . .
O23 P1 O20 111.2(2) . .
O11 P1 O20 112.1(2) . .
O23 P1 C1 107.9(3) . .
O11 P1 C1 108.6(2) . .
O20 P1 C1 108.2(2) . .
O23 P1 Li1 87.6(2) . 2_565
O11 P1 Li1 34.9(2) . 2_565
O20 P1 Li1 147.0(3) . 2_565
C1 P1 Li1 90.1(3) . 2_565
O13 P2 O1 114.0(3) . .
O13 P2 O10 111.3(2) . .
O1 P2 O10 107.1(2) . .
O13 P2 C2 110.8(3) . .
O1 P2 C2 106.2(2) . .
O10 P2 C2 107.0(2) . .
O13 P2 Li1 134.7(3) . .
O1 P2 Li1 40.0(2) . .
O10 P2 Li1 67.5(2) . .
C2 P2 Li1 112.5(3) . .
O16 P3 O7 112.9(2) . .
O16 P3 O12 111.9(2) . .
O7 P3 O12 109.2(2) . .
O16 P3 C2 109.0(2) . .
O7 P3 C2 106.1(2) . .
O12 P3 C2 107.4(2) . .
O17 P4 O3 114.7(3) . .
O17 P4 O19 106.7(3) . .
O3 P4 O19 110.2(3) . .
O17 P4 C1 108.0(3) . .
O3 P4 C1 111.0(3) . .
O19 P4 C1 105.7(3) . .
O17 P4 Li3 33.6(3) . 2_665
O3 P4 Li3 92.2(3) . 2_665
O19 P4 Li3 140.2(3) . 2_665
C1 P4 Li3 95.6(3) . 2_665
O17 P4 Li1 146.5(3) . 2_565
O3 P4 Li1 31.8(2) . 2_565
O19 P4 Li1 93.1(3) . 2_565
C1 P4 Li1 91.5(3) . 2_565
Li3 P4 Li1 120.0(3) 2_665 2_565
O27 P5 O15 111.5(3) . .
O27 P5 O5 111.1(3) . .
O15 P5 O5 108.3(2) . .
O27 P5 C3 111.9(3) . .
O15 P5 C3 106.6(3) . .
O5 P5 C3 107.3(3) . .
O29 P6 O14 109.6(3) . .
O29 P6 O21 111.8(3) . .
O14 P6 O21 109.8(2) . .
O29 P6 C3 110.9(3) . .
O14 P6 C3 108.4(3) . .
O21 P6 C3 106.1(3) . .
O29 P6 Li4 33.3(4) . 2_566
O14 P6 Li4 79.6(4) . 2_566
O21 P6 Li4 138.3(4) . 2_566
C3 P6 Li4 108.9(4) . 2_566
P2 O1 Li1 111.6(3) . .
P2 O1 Mo1 130.0(2) . .
Li1 O1 Mo1 102.5(3) . .
Mo2 O2 Mo4 82.39(15) . .
P4 O3 Li1 123.6(4) . 2_565
P5 O5 Mo4 137.0(2) . .
Mo1 O6 Mo3 82.70(15) . .
P3 O7 Mo2 130.5(2) . 2_565
Mo1 O8 Mo3 82.45(15) . .
Mo2 O9 Mo4 82.50(15) . .
P2 O10 Mo2 127.8(2) . 2_565
P1 O11 Li1 119.5(4) . 2_565
P1 O11 Mo2 122.0(2) . .
Li1 O11 Mo2 111.0(3) 2_565 .
P3 O12 Mo1 128.2(2) . .
P2 O13 Li2 143.3(5) . 1_565
P6 O14 Mo4 136.9(2) . .
P5 O15 Mo3 137.6(2) . .
P3 O16 Li3 145.2(5) . .
P3 O16 Li2 130.2(4) . 2_665
Li3 O16 Li2 80.9(5) . 2_665
P4 O17 Li2 151.3(5) . .
P4 O17 Li3 120.7(5) . 2_665
Li2 O17 Li3 84.6(6) . 2_665
P1 O20 Mo4 116.7(2) . .
P6 O21 Mo3 135.0(2) . .
P1 O23 Li1 130.6(4) . .
P1 O23 Mo1 122.7(2) . .
Li1 O23 Mo1 102.2(4) . .
P5 O27 Li6 145.1(8) . .
P5 O27 Li7 138.9(16) . .
Li6 O27 Li7 38.5(16) . .
P6 O29 Li4 121.4(7) . 2_566
P4 C1 P1 118.2(3) . .
P4 C1 H1A 107.8 . .
P1 C1 H1A 107.8 . .
P4 C1 H1B 107.8 . .
P1 C1 H1B 107.8 . .
H1A C1 H1B 107.1 . .
P2 C2 P3 113.4(3) . .
P2 C2 H2A 108.9 . .
P3 C2 H2A 108.9 . .
P2 C2 H2B 108.9 . .
P3 C2 H2B 108.9 . .
H2A C2 H2B 107.7 . .
P6 C3 P5 111.5(3) . .
P6 C3 H3A 109.3 . .
P5 C3 H3A 109.3 . .
P6 C3 H3B 109.3 . .
P5 C3 H3B 109.3 . .
H3A C3 H3B 108.0 . .
Li7 OW1 Li6 39.5(18) 2_576 2_576
Li5 OW6 Li7 127.0(16) 1_545 2_566
Li7 OW8 Li6 39.5(18) 2_676 2_676
OW15 OW11 Li5 59.9(15) . .
OW14 OW13 Li5 67.5(14) . 2_676
OW13 OW14 Li5 70.4(15) . 2_676
OW11 OW15 Li5 92.5(17) . .
O3 Li1 O23 124.9(6) 2_565 .
O3 Li1 O11 97.8(5) 2_565 2_565
O23 Li1 O11 124.8(5) . 2_565
O3 Li1 O1 105.3(5) 2_565 .
O23 Li1 O1 81.1(4) . .
O11 Li1 O1 122.9(5) 2_565 .
O3 Li1 P2 103.2(4) 2_565 .
O23 Li1 P2 104.9(4) . .
O11 Li1 P2 96.0(4) 2_565 .
O1 Li1 P2 28.41(18) . .
O3 Li1 P4 24.6(2) 2_565 2_565
O23 Li1 P4 149.2(5) . 2_565
O11 Li1 P4 76.3(3) 2_565 2_565
O1 Li1 P4 107.2(4) . 2_565
P2 Li1 P4 93.5(3) . 2_565
O3 Li1 P1 76.9(4) 2_565 2_565
O23 Li1 P1 128.5(5) . 2_565
O11 Li1 P1 25.53(19) 2_565 2_565
O1 Li1 P1 143.2(4) . 2_565
P2 Li1 P1 114.8(3) . 2_565
P4 Li1 P1 60.2(2) 2_565 2_565
O3 Li1 Mo1 125.3(5) 2_565 .
O23 Li1 Mo1 42.1(2) . .
O11 Li1 Mo1 134.7(5) 2_565 .
O1 Li1 Mo1 39.1(2) . .
P2 Li1 Mo1 63.7(2) . .
P4 Li1 Mo1 140.2(4) 2_565 .
P1 Li1 Mo1 157.8(4) 2_565 .
O3 Li1 Li1 96.2(5) 2_565 2_565
O23 Li1 Li1 72.6(4) . 2_565
O11 Li1 Li1 69.3(4) 2_565 2_565
O1 Li1 Li1 152.6(6) . 2_565
P2 Li1 Li1 157.2(5) . 2_565
P4 Li1 Li1 99.4(5) 2_565 2_565
P1 Li1 Li1 58.0(3) 2_565 2_565
Mo1 Li1 Li1 113.9(4) . 2_565
O17 Li2 O13 111.5(6) . 1_545
O17 Li2 OW3 106.1(7) . 1_545
O13 Li2 OW3 108.9(6) 1_545 1_545
O17 Li2 O16 94.6(5) . 2_665
O13 Li2 O16 122.8(7) 1_545 2_665
OW3 Li2 O16 111.1(6) 1_545 2_665
O17 Li2 Li3 48.2(4) . 2_665
O13 Li2 Li3 136.0(7) 1_545 2_665
OW3 Li2 Li3 114.2(6) 1_545 2_665
O16 Li2 Li3 46.6(4) 2_665 2_665
O16 Li3 O17 99.3(6) . 2_665
O16 Li3 O28 116.3(7) . 2_665
O17 Li3 O28 112.4(7) 2_665 2_665
O16 Li3 O25 109.9(7) . 2_665
O17 Li3 O25 105.7(6) 2_665 2_665
O28 Li3 O25 112.1(6) 2_665 2_665
O16 Li3 Li2 52.4(4) . 2_665
O17 Li3 Li2 47.2(4) 2_665 2_665
O28 Li3 Li2 125.1(7) 2_665 2_665
O25 Li3 Li2 122.2(6) 2_665 2_665
O16 Li3 P4 123.2(6) . 2_665
O17 Li3 P4 25.7(2) 2_665 2_665
O28 Li3 P4 104.6(5) 2_665 2_665
O25 Li3 P4 87.3(4) 2_665 2_665
Li2 Li3 P4 72.2(4) 2_665 2_665
OW10 Li4 O29 102.4(10) 1_455 2_566
OW10 Li4 OW4 103.6(11) 1_455 .
O29 Li4 OW4 110.2(11) 2_566 .
OW10 Li4 OW7 109.9(11) 1_455 .
O29 Li4 OW7 127.2(11) 2_566 .
OW4 Li4 OW7 101.5(9) . .
OW10 Li4 P6 122.4(9) 1_455 2_566
O29 Li4 P6 25.3(3) 2_566 2_566
OW4 Li4 P6 114.8(8) . 2_566
OW7 Li4 P6 102.8(8) . 2_566
OW15 Li5 OW14 72.1(14) . 2_676
OW15 Li5 OW5 107.2(12) . .
OW14 Li5 OW5 109.6(14) 2_676 .
OW15 Li5 OW6 126.3(15) . 1_565
OW14 Li5 OW6 120.8(14) 2_676 1_565
OW5 Li5 OW6 113.9(14) . 1_565
OW15 Li5 OW13 114.0(15) . 2_676
OW14 Li5 OW13 42.1(10) 2_676 2_676
OW5 Li5 OW13 99.8(13) . 2_676
OW6 Li5 OW13 91.7(11) 1_565 2_676
OW15 Li5 OW11 27.6(7) . .
OW14 Li5 OW11 96.0(15) 2_676 .
OW5 Li5 OW11 112.5(12) . .
OW6 Li5 OW11 102.3(12) 1_565 .
OW13 Li5 OW11 135.0(15) 2_676 .
Li7 Li6 O27 78(3) . .
Li7 Li6 OW1 66(3) . 2_576
O27 Li6 OW1 107.4(11) . 2_576
Li7 Li6 OW8 65(3) . 2_676
O27 Li6 OW8 114.5(11) . 2_676
OW1 Li6 OW8 103.8(11) 2_576 2_676
Li7 Li6 OW12 164(3) . 2_676
O27 Li6 OW12 117.8(12) . 2_676
OW1 Li6 OW12 103.7(11) 2_576 2_676
OW8 Li6 OW12 108.1(11) 2_676 2_676
Li6 Li7 OW8 76(3) . 2_676
Li6 Li7 OW1 75(3) . 2_576
OW8 Li7 OW1 114(3) 2_676 2_576
Li6 Li7 O27 63(2) . .
OW8 Li7 O27 112(3) 2_676 .
OW1 Li7 O27 105(3) 2_576 .
Li6 Li7 OW6 173(4) . 2_566
OW8 Li7 OW6 108(3) 2_676 2_566
OW1 Li7 OW6 98(2) 2_576 2_566
O27 Li7 OW6 120(3) . 2_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O4 1.700(4) .
Mo1 O8 1.945(4) .
Mo1 O6 1.947(4) .
Mo1 O12 2.125(4) .
Mo1 O1 2.126(4) .
Mo1 O23 2.255(4) .
Mo1 Mo3 2.5760(6) .
Mo1 Li1 3.289(11) .
Mo2 O22 1.700(4) .
Mo2 O2 1.946(4) .
Mo2 O9 1.949(4) .
Mo2 O7 2.121(4) 2_565
Mo2 O10 2.137(4) 2_565
Mo2 O11 2.231(4) .
Mo2 Mo4 2.5751(6) .
Mo3 O18 1.678(4) .
Mo3 O6 1.952(4) .
Mo3 O8 1.964(4) .
Mo3 O15 2.068(4) .
Mo3 O21 2.096(4) .
Mo4 O26 1.679(5) .
Mo4 O9 1.957(4) .
Mo4 O2 1.963(4) .
Mo4 O5 2.076(4) .
Mo4 O14 2.077(4) .
Mo4 O20 2.468(4) .
P1 O23 1.539(4) .
P1 O11 1.542(4) .
P1 O20 1.549(4) .
P1 C1 1.808(6) .
P1 Li1 3.113(11) 2_565
P2 O13 1.499(4) .
P2 O1 1.548(4) .
P2 O10 1.557(4) .
P2 C2 1.803(5) .
P2 Li1 3.025(11) .
P3 O16 1.507(4) .
P3 O7 1.549(4) .
P3 O12 1.552(4) .
P3 C2 1.805(5) .
P4 O17 1.510(4) .
P4 O3 1.535(5) .
P4 O19 1.595(5) .
P4 C1 1.806(5) .
P4 Li3 2.996(12) 2_665
P4 Li1 3.069(10) 2_565
P5 O27 1.499(4) .
P5 O15 1.545(4) .
P5 O5 1.546(4) .
P5 C3 1.810(6) .
P6 O29 1.511(5) .
P6 O14 1.542(4) .
P6 O21 1.552(4) .
P6 C3 1.799(6) .
P6 Li4 3.019(19) 2_566
O1 Li1 2.091(12) .
O3 Li1 1.942(11) 2_565
O7 Mo2 2.121(4) 2_565
O10 Mo2 2.137(4) 2_565
O11 Li1 2.049(11) 2_565
O13 Li2 1.907(12) 1_565
O16 Li3 1.896(13) .
O16 Li2 2.067(14) 2_665
O17 Li2 1.898(12) .
O17 Li3 1.930(13) 2_665
O23 Li1 1.965(10) .
O25 Li3 2.010(14) 2_665
O27 Li6 1.87(2) .
O27 Li7 2.04(5) .
O28 Li3 1.986(14) 2_665
O29 Li4 1.94(2) 2_566
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
OW1 Li7 1.86(5) 2_576
OW1 Li6 1.97(2) 2_576
OW3 Li2 2.007(15) 1_565
OW4 Li4 1.96(2) .
OW5 Li5 1.97(2) .
OW6 Li5 1.98(3) 1_545
OW6 Li7 2.18(6) 2_566
OW7 Li4 2.05(2) .
OW8 Li7 1.85(5) 2_676
OW8 Li6 1.98(2) 2_676
OW10 Li4 1.84(2) 1_655
OW11 OW15 1.00(2) .
OW11 Li5 2.16(3) .
OW12 Li6 1.98(2) 2_676
OW13 OW14 1.41(3) .
OW13 Li5 1.98(3) 2_676
OW14 Li5 1.94(4) 2_676
OW15 Li5 1.87(3) .
Li1 O3 1.942(11) 2_565
Li1 O11 2.049(11) 2_565
Li1 P4 3.069(10) 2_565
Li1 P1 3.113(11) 2_565
Li1 Li1 3.44(2) 2_565
Li2 O13 1.907(12) 1_545
Li2 OW3 2.007(15) 1_545
Li2 O16 2.067(14) 2_665
Li2 Li3 2.576(17) 2_665
Li3 O17 1.930(13) 2_665
Li3 O28 1.986(14) 2_665
Li3 O25 2.010(14) 2_665
Li3 Li2 2.576(17) 2_665
Li3 P4 2.996(12) 2_665
Li4 OW10 1.84(2) 1_455
Li4 O29 1.94(2) 2_566
Li4 P6 3.019(19) 2_566
Li5 OW14 1.94(4) 2_676
Li5 OW6 1.98(3) 1_565
Li5 OW13 1.98(3) 2_676
Li6 Li7 1.30(6) .
Li6 OW1 1.97(2) 2_576
Li6 OW8 1.98(2) 2_676
Li6 OW12 1.98(2) 2_676
Li7 OW8 1.85(5) 2_676
Li7 OW1 1.86(5) 2_576
Li7 OW6 2.18(6) 2_566
